Upcoming SlideShare
×

# Reader materials and structures: 11. Fatigue & Durability

• 224 views

• Comment goes here.
Are you sure you want to
Be the first to comment
Be the first to like this

Total Views
224
On Slideshare
0
From Embeds
0
Number of Embeds
1

Shares
8
0
Likes
0

No embeds

### Report content

No notes for slide

### Transcript

• 2. Introduction to Aerospace Engineering – Structures and Materials11.2 Stress and strain concentrations11.2.1 DefinitionFollowing from the definitions provided in chapter 1, the stress in a material or component is basicallycalculated by dividing the applied force by the area. Or in equation form F σ= (11.1) AThis is considered correct if the material is homogeneous and in undisturbed in shape or geometry.This concept is illustrated in Figure 11.1. Independent on where a cross-section is considered, thestresses will be equal and evenly distributed through the material. These stresses can be calculatedwith equation (11.1). Figure 11.1 Illustration of evenly distributed stresses in a homogeneous materialHowever, of the geometry or the shape is changed, or if a cut, damage or crack is created in thematerial, then this forms a disturbance for the stress field. The load that has to be transferred throughthe material, illustrated in Figure 11.2 with stress lines, has to bypass the cut or damage. Homogeneous stress field Stress field with disturbance Figure 11.2 Comparison between evenly distributed stress field (left) and a disturbed stress field (right)170
• 3. 11 Fatigue & DurabilityAssuming that equation (11.1) is still valid, one should at the location of the disturbance calculate thestress by dividing the applied load F by the reduced cross section. Because the cross-sectional area isreduced while the load remains the same, this implies that the stress at the location of the disturbanceis higher than in the undisturbed stress field. This higher stress is generally denoted as the nominalstress and is defined by F A F A σ nom = * = * = *σ (11.2) A A A A grossThis would suggest that if the failure of a disturbed or cracked component has to be predicted, onemay assume that once the nominal stress σnom equals ultimate strength of the material, failure wouldoccur. However, before this equilibrium has been reached, the material or component will fail.This phenomenon is related to the fact that a concentration of stress is present at the tip of the notch.This is illustrated with the higher density of stress lines at the notch tip in Figure 11.2. The undisturbedand evenly distributed stress field has to bypass the notch, which at the location of the end of the notchcreates a high concentration of stress. This phenomenon is indicated with the term stressconcentration.To evaluate the stress concentration, a stress concentration factor Kt has been defined σ peak K = (11.3) t σ nomHere the peak stress is the highest stress right at the edge or tip of the notch and the nominal stressσnom is calculated with equation (11.2). σapplied σnom σapplied D W σpeak Figure 11.3 Example of a flat sheet containing a hole loaded by a far field stressConsider a flat panel with width W containing a circular hole with diameter D, see Figure 11.3, thenominal stress can be calculated with 171
• 4. Introduction to Aerospace Engineering – Structures and Materials Wσ nom = σ (11.4) W − D appliedThe stress concentration factor can then be calculated with equation (11.3). The only question at thispoint will be whether the peak stress is known. Because people in the past did not have the availabilityof dedicated software that can be used to calculate stresses at specific locations for any geometryunder load, like with for example Finite Element Software, theoretical solutions were mathematicallyderived. These theoretical solutions were derived for the case of notches in sheets with infinitedimensions, because mathematically the boundary constraints for this case are exactly known.For the finite geometries, subsequently correction factors were determined based upon calculations orexperimental data. These solutions were combined in handbooks, like for example Peterson’s Stressconcentration factors [1].A well-known general solution for an elliptical hold in an infinite sheet illustrated in Figure 11.4 isgiven by σ peak a a K = = 1+ 2 = 1+ 2 (11.5) t σ nom b rThis means that the stress concentration factor for a circular hole in an infinite sheet is equal to Kt = 3.This value is indifferent from the hole diameter! The relation between the peak stress at the notch andthe nominal stress in the remaining cross-section section remains 3, independent what hole diameter isconsidered. r 2b 2a Figure 11.4 Illustration of an elliptical hole in an axially loaded infinite sheet172
• 5. 11 Fatigue & DurabilityAn important remark has to be made. When introducing the stress concentration factor Kt and the peakstress at the notch edge, it was argued that the component would fail before the nominal stress σnomwould have reached the ultimate strength of the material.Implicitly, this explanation and subsequent derivation may lead to the assumption that failure wouldthus occur when the peak stress σpeak reaches the ultimate strength. This is correct for materials thatremain (approximately) linear elastic until failure, like for example fibre reinforced polymercomposites.However, metallic materials usually plastically deform beyond the yield strength. In that case thebehaviour will be different. This is illustrated in Figure 11.5. The stiffness of material reducessignificantly beyond yielding (evident from the tangent slope compared to the linear elastic slope,represented by the Young’s modulus E). As a result of this local stiffness reduction, stress will beredistributed to the remaining material. Figure 11.5 Effect of elastic-plastic material behaviour on the stress concentrationThe example given on the next page, illustrates that linear elastic materials have significant highernotch sensitivities than ductile materials. As a result, the failure strength of a notched component madeof linear elastic materials is usually lower than that of equivalent elastic-plastic materials.On the other hand, as will be discussed later in this chapter, composites are usually less sensitive tofatigue loads. In other words, comparing aerospace aluminium alloys with carbon fibre composites,one may conclude that stress concentrations are detrimental for static loads on composites anddetrimental for fatigue loads in aluminium alloys.11.2.2 Saint Venant’s principleAn important principle for structural analysis is the principle of Saint Venant. This principle states thatthe effect of a local disturbance, due to for example a notch, remains limited to the direct neighbour-hood of the location of that notch, see Figure 11.6. 173
• 6. Introduction to Aerospace Engineering – Structures and Materials Example: Effect of plasticity on Kt Consider a straight sample containing a hole, as illustrated in Figure 11.5. If the material behaviour would be linear elastic until failure, like for example carbon fibre composite, this sample would fail when σpeak = σult, which means that the gross strength of failure is equal to W −D σ σ applied = σ nom = ult W K t For a sheet with infinite dimensions, this means that the failure strength is equal to σult/3. For isotropic carbon fibre composite the failure strength can be about 500 MPa, which means that failure of the sample would occur at 166 MPa. If the material behaviour would be elastic-plastic like for example aluminium W −D σ applied = σ nom ≈ 0.9 σ ult W For a sheet with infinite dimensions, this means that the failure strength is equal to about 0.9 σult. With the failure strength of aluminium 2024-T3 of about 450 MPa, this implies failure would occur at about 405 MPa. Do consider however that the density of aluminium 2024-T3 is about 2.7 g/cm3 (providing a specific failure strength of 150 kN⋅m/kg), while the carbon fibre composite would be about 1.5 g/cm3 (thus a specific strength of 110 kN⋅m/kg) . 5 elliptical hole; a/b = 3 4 3 circular hole 2 1 y σy S x a 2a 3a ~3DFigure 11.6 Illustration of Saint Venant’s principle: Stress disturbance due to a notch remains limited to the direct neighbourhood of the notch174
• 7. 11 Fatigue & DurabilityThe benefit of this principle is that the stress analysis of a loaded structure can be divided into a - global stress analysis (considering the structure as a whole) - local stress analysis of all details (containing notches)This approach is justified by the Saint Venant’s principle; a structure faces the same stresses due toapplied loading indifferent of the presence of a notch at a certain location, except for the location ofthe notch itself.11.2.3 Stress distribution around a holeFor the sake of simplicity, the stress concentration factor Kt has been introduced while limiting thediscussion to the stress in the net section (nominal stress) and the stress at the notch edge (peak stress).However, it is obvious that the disturbance in stress created by the presence of the notch is somewhatmore complex. The peak stress described by Kt is only at the location in the net section. Away from thehole edge or along the contour of the notch, the stresses reduce and may even become negative.This is illustrated in Figure 11.7. In this figure a peak stress of 3S is present at both sides of the hole,while a compressive stress is present at the locations given by ϕ=±π/2. This compressive stress may beunderstood when considering the stress lines similar to the ones illustrated in Figure 11.2. Thesestresses may be decomposed in stresses in horizontal and vertical direction, where the horizontalcomponent just above and below the hole induce a compressive stress. S Kt = 3 0.9 σ σ S 0.9 σ y σφ 0.28 mm φ x 0.043 mm ~ ρ = 1 mm grain size 3SFigure 11.7 Illustrations of the tangential stress distribution around a hole in an infinite sheet; tensile peak stress at ϕ=0,π changes to compressive stress at ϕ=±π/2 (left); drop in stress away from the hole is more severe than along the notch contour.Another aspect that can be observed in Figure 11.7 is that the stress drops quickly moving away fromthe hole, while the drop along the contour is significantly less. This implies there is a certain areaalong the notch contour that may be considered relatively high stressed (in the order of 0.9σ), wherepotentially fatigue cracks may initiate. 175